**ABSTRACT **

HEWITT, ANDREW SCOTT. Coupling Organic Molecules to Topological Insulators. (Under the direction of Dr. Daniel Dougherty.)

Macroscopic systems displaying quantum behavior can be investigated to gain insights into the fundamental nature of our universe. Topological insulators (TIs) are a recent example of such systems exhibiting exotic physical phenomenon in condensed matter. These topologically nontrivial materials are bulk insulating and have spin-momentum locked surface states as a result of its interface with a normal insulator. The topological surface states (TSS) are guaranteed by the materials topological invariant, and for materials studied in this thesis, protected by time-reversal symmetry (TRS). The TSS exist in ambient conditions with no need for external applied fields allowing investigations of its nature relatively easy and obvious interest for spintronic devices. Organic molecules represent an electronic and magnetic knob by which one can tune the properties of the substrate of interest and are also of interest for spintronic applications. The organic-TI interface is a new unexplored playground to observe and probe novel physics.

The surface is a unique environment for each solid and must be characterized by surface sensitive techniques. Prototypical TIs of study have been the van der Waals (vdW) layered binary chalcogenides. Characterization of the surface of cleaved Bi2Se3 samples by X-ray photoemission spectroscopy (XPS) and angle-resolved photoemission spectroscopy (ARPES) show that coexisting surface terminations are probable if performed in air, while in-situ cleaves are terminated as expected along a vdW layer. The electronic structure depends on the surface termination illustrating the important question of surface effects on the TSS.

Breaking TRS in these systems is predicted to result in the quantum anomalous hall effect and topological magnetoelectric effects. Ferromagnetic TIs are expected to have a gapped TSS that can be measured by ARPES. We investigated bulk Cr-doping of the TI Bi1.5Sb0.5Te1.7Se1.3 (BSTS) studied by XPS and ARPES. Low-doped samples have detectable concentrations of Cr near the surface, however higher-doped samples show no evidence for Cr-dopants. Powder x-ray diffraction shows CrxSey impurities in higher Cr-doped samples. This suggests that phase segregation is likely occurring and represents the general limitation of bulk-doping.

Coupling Organic Molecules to Topological Insulators

by

Andrew Scott Hewitt

A dissertation submitted to the Graduate Faculty of North Carolina State University

in partial fulfillment of the requirements for the degree of

Doctor of Philosophy

Physics

Raleigh, North Carolina 2016

APPROVED BY:

_______________________________ _______________________________

Dr. Daniel B. Dougherty Dr. Kenan Gondogdu

Committee Chair

_______________________________ _______________________________

Dr. Paul A. Maggard Dr. Laura Clarke

ii

**DEDICATION **

iii

**BIOGRAPHY **

iv

**ACKNOWLEDGMENTS **

I’d like to thank my family for their love and support throughout my life and this journey. My mom has always encouraged me to push myself to be a better person and student. My dad inspired me to pursue a career in science from a young age. My brother and sister have always provided love and support through the roller-coaster of emotions that is the graduate school experience. Without your support I would not have been able to succeed.

My friends in physics and in the Dougherty group have also provided much support and

guidance. Jingying helped to train me on the STM and spent long hours acquiring data by my side in the lab. She has a solid understanding of surface science physics and great insight. I’d also like to thank Terry for inspiring me to be the best possible scientist I can be. From helping me fixing my car numerous times, displaying his brilliance for the scientific process, and convincing me to continue for my Ph.D., I couldn’t have done this without your friendship. Ben, Matt, and Jon have also provided support during this process as well as many good jam sessions.

v

**TABLE OF CONTENTS **

List of Figures………...vii

**Chapter 1 Topological Insulators………...1 **

1.1 Introduction to Topological Insulators…………...………1

1.2 Crystallography Background……….……..………..2

1.3 Tight-Binding Model …...………..………...3

1.4 Topological Band Theory ……...………..………..………..5

1.5 Model Hamiltonian for Binary TIs………..………..………..11

1.6 Experimental Evidence for 3D Topological Insulators………..……….…….14

1.7 Breaking Time-Reversal Symmetry………..………..15

1.8 Surface Science Challenges for TI Research………..………….16

1.9 Molecular-Orbital Theory………..………..18

1.10 Survey of the Organic-TI interface………..………..…………21

References………...………23

**Chapter 2 Experimental Methods………28 **

2.1 Surface Science……….………28

2.2 Photoelectron Spectroscopy Theory……….32

2.3 Photoelectron Spectroscopy Experiment and Equipment……….35

2.4 Scanning Tunneling Microscopy/Spectroscopy………...………37

References………...…39

**Chapter 3 Coexisting Bi and Se Terminated Surfaces of Cleaved Bi2Se3 Crystals………..41 **

3.1 Preface………..……41

**Chapter 4 Cr-doping of the topological insulator Bi1.5Sb0.5Te1.7Se1.3 ………54 **

4.1 Preface………...……54

4.2 Materials Science Challenges in TI Synthesis……….………….55

4.3 Experimental Methods………..………57

4.4 Structural Details……….…...57

4.5 Chemical Composition……….60

4.6 Electronic Structure………..62

4.7 Magnetic and Electronic Transport Properties ………..……..……….…63

4.8 Conclusions………..………...……..65

References………...…66

vi

5.1 Introduction………...………71

5.2 Experimental Methods………..………72

5.3 Results……….………..72

5.4 Conclusions………...………78

vii

**LIST OF FIGURES **

Figure 1.1 Cartoon picture of an electronic state confined to the surface of a material (left) which decays exponentially into the bulk and vacuum. The topological invariant must change at the surface of a TI which closes the energy gap resulting in the spin-textured

TSS……….……….. 10 Figure 1.2 (a) Schematic of the bulk bands and TSS showing the forbidden backscattering where an

electron at k*i* must flip its spin to transition to -k*i*. (b) The hexagonal surface BZ of the
strong 3D TIs studied in this thesis with symmetry points indicated. The purple circle
represents Fermi surface of the Dirac cone with spin locked perpendicular to its

momentum... 11 Figure 1.3 Crystal structure of layered binary TIs showing the unit cell and QL stacking (a). The

hexagonal (111) atomic surface representative of the crystal termination for a perfect cleave (b).……….. ……….. 13 Figure 1.4 Crystal structure of layered binary TIs showing the unit cell and QL stacking (a). The

hexagonal (111) atomic surface representative of the crystal termination for a perfect cleave (b).……….. ………18 Figure 1.5 Schematic drawing of atomic orbitals s, p, and d and their symmetry………..19 Figure 1.6 (a) sigma bond formed by overlap of an s and p orbital. (b) Zero overlap between s and p

orbitals resulting in no bond. (c) pi-bond formed by the overlap of two p

orbitals………20 Figure 1.7 The D4h symmetry elements for the MPc molecule are shown. The highest symmetry is

the four-fold rotation (C4) around the central metal atom (blue arrow) defining the principal axis. The six two-fold rotations (C2) are in the plane of the molecule (red lines). The σh plane is perpendicular to the principal axis which is in the plane of the molecule. The mirror-symmetry planes (black lines) are given by σv and σd where σv intersects the greater number of atoms……….. ……… 21 Figure 1.8 MnPc molecule and the ordering of its d-shell according to ligand-field theory. The

filling of these orbitals is shown for thin films as measured by Bromboui et

*al……….22 *
Figure 2.1 Annealing a Cr-crystal in the UHV STM chamber………..……. 28
Figure 2.2 Illustration of gas particles and adsorbates on a surface………..……….. 30
Figure 2.3 Synthesized Bi2Te3 crystals by Jonathon Boltersdorf in the Maggard chemistry group at

viii and are on the order of a few mm. Atomic resolution of a step-edge for a vacuum cleaved crystal where triangular subsurface defects can be seen………31 Figure 2.4 Box chamber diagram of OMBD. A sample is mounted near the QCM flux monitor and

sublimed molecules spray from a quartz crucible heated by a Ta-wire……….32 Figure 2.5 (a) Cylindrical mirror analyzer illustration showing the two stages and electron trajectory. The beams of photoelectrons are focused on an electron multiplier recording the number of counts per second. The higher resolution hemispherical analyzer (b) containing an electrostatic lens used to discriminate the entrance of photoelectrons according to their kinetic energy……….………...………36 Figure 2.6 Illustration of STM tip, controls, and sample. In constant current mode, a bias is applied

between the tip and sample and the height of the tip is recorded and adjusted to maintain
a given tunneling current. An example of the atomic resolution achievable in these
systems is given for a Bi2Te3 sample………38
Figure 4.1 (a) Crystal structure of the Bi1.5-*x*Cr*x*Sb0.5Te1.7Se1.3 solid solution comprised of quintuple

layers. (b) A view along the c-axis of the hexagonal layers is outlined in black, and the magenta, yellow, and green spheres represent the Bi/Sb/Cr, Te, and Se atoms,

respectively…...……….58 Figure 4.2 Powder X-ray diffraction pattern calculated from the crystal structure of

Bi1.5Sb0.5Te1.7Se1.3 (BSTS) and experimental patterns of pure 0-20% Cr-doped BSTS crystals. The most intense peaks are labeled with their Miller indices (hkl) on the

calculated patterns...…….………..…59 Figure 4.3 PXRD of the 20% Cr-BSTS sample showing the top (green), middle (blue), and bottom

(pink) of the single crystal. Calculated PXRD patterns are shown for BSTS (black) and
Cr0.68Se (red). The Cr0.68Se impurity is observed to segregate to the top of the crystal, and
no residual impurity is observed in the middle or bottom of the crystal………...60
Figure 4.4 XPS of the Te 3d and Cr 2p core levels for 0%-4% Cr-BSTS **(a) **and 7%-20% **(b). **A

small but detectable amount of Cr is seen in the 0.25% Cr-BSTS (red) and grows in intensity for the 1% and 4% Cr-BSTS. The Cr 2p peak is noticeably absent in the higher doped samples…..……….………....……….61 Figure 4.5 XPS spectra of Sb 3d and O 1s core levels for 0%, 0.25%, 1%, and 4% Cr-BSTS. A

strong doublet peak is observed for all samples for the spin-split Sb 3d state. A noticeable amount of oxygen contamination is observed for the 1% Cr-BSTS (orange

ix Figure 4.6 UPS at the Γ-point for 0% (black) and 4% (blue). A clear shift towards higher binding

energy is observed for the BVB for the 4% Cr sample…...………63 Figure 4.7 Resistivity (mΩ cm) as a function of temperature (K) for 0%, 0.25%, 1%, and 4%

Cr-BSTS (a, b, c, and d respectively). An upward turn in resistivity is observed for all samples below ~75 K indicative of an insulating ground state. The 1% Cr-BSTS is an anomaly showing metallic behavior before transitioning to the insulating

state………..………...64 Figure 4.8 Magnetization (emu/gm) as a function of temperature (K) for the 0%, 0.25%, 1%, and 4%

Cr-BSTS (a, b, c, and d). The gentle upslope in the 0%, 0.25%, and 1% indicates a diamagnetic response. The 4% Cr-BSTS sample has a peak indicating an

antiferromagnetic phase transition around 50 K………..65
Figure 5.1 ARPES maps of clean (a), ~0.13 Mol/nm2_{ (b), and ~0.28 Mol/nm}2_{ (c) with Fermi level }

indicated by dashed white line. The well-known M-shape of the bulk valence band of
Bi2Te3 is clearly seen as well as the TSS indicating the Fermi level falls in the bulk gap.
The bulk conduction band is observed at Ef after depositing of ~0.13 Mol/nm2_{ of MnPc }
(b) consistent with previous reports of n-doping. Increasing the molecular coverage
reveals a new hybrid-interface state emerging at 0.4 eV below Ef.…………...………73
Figure 5.2 ARPES maps of clean (a), ~0.13 Mol/nm2_{ (b), and ~0.28 Mol/nm}2_{ (c) with Fermi level }

indicated by dashed white line. The bulk bands can clearly be seen dispersing with a
maximum intensity at 0.8 eV for the Γ-point at 0.0 Å-1_{ and an M-shape at the top of the }
BVB. The appearance of the MnPc molecular orbitals (Mos) can be seen after depositing
~0.13 Mol/nm2_{ (b). The BCB can also be seen as the MnPc molecules n-dope Bi2Te3. }
Increasing the molecular coverage to ~0.28 Mol/nm2_{ (c) reveals a new hybrid-interface }
state emerging at 0.4 eV below Ef along with an increase in intensity and decrease in
dispersion of the MnPc MOs.………..…...………..…74
Figure 5.3 Normal emission (k||=0 (Å-1_{)) for the clean and molecule-covered surfaces (a) showing }

x Figure 5.4 STM of MnPc on Bi2Te3 for different coverages. The initial growth (a) consists of

disperse molecules with some tendency to form chains indicated by white dashed lines. Increasing the coverage reveals previously unobserved close-packed structures (b). AFM shows islands forming at higher coverages (c)…..………..76 Figure 5.5 STS dI/dV spectra of MnPc/Bi2Te3 system on (red) and off (black) the molecule. The

1

**CHAPTER 1 TOPOLOGICAL INSULATORS **

**1.1 Introduction to Topological Insulators **

Technology in our everyday life mainly consists of electronic devices in which electrical current is used to operate a device, however, it was only recently discovered that spin-dependent phenomena can be realized in functional devices.[3] Memory devices (i.e. hard disk drives) rely on a change in the resistance of sandwiched ferromagnetic thin films to store information. This represents a pardigm shift to exploit the quantum mechanical nature of spin. Of course, to operate and build logic circuits to make use of this phenomenon electrical current is needed. It was unveiled in the past decade that there exists a class of materials which harbor spin-textured gapless surface states on a bulk insulating material existing in ambient conditions with no external magnetic field required as guaranteed by the materials topological invariant.[4, 5] These topological insulators (TIs) are a promising candidate for low power consumption devices (e.g. transistors).[6, 7] Experiments on their spin to charge current conversion efficiency and spin polarization have shown their promise for spintronic devices[8, 9], in addition to theoretical and

experimental work showing controlled functionality of topological states with an electric field.[10, 11] Furthermore, exotic phenomena such as the magnetic monopole and majorana fermions have been predicted to be observable in TI systems.[12, 13]

TIs are a condensed matter phenomenon that was first discovered in the 1980s in the
two-dimensional (2D) integer and fractional quantum hall states.[14] These materials are manifestations of
topological invariants which protect their edge states such that the quantization of the Hall conductivity
has been measured to 1 part in 109_{ and are physically understood in terms of its Berry phase.[5, 15] It is }
interesting and worth noting that the Berry phase was first discovered for quantum adiabatic transport of
particles in a slowly varying applied field before later being applied to Bloch wave functions.

While the integer quantum hall effect (IQHE) requires an external magnetic field to be applied in order to observe the edge states, the experimental discovery of the spin hall effect, transverse spin current under an electric field, in nonmagnetic systems in 2004 was a turning point in topological condensed matter community.[16] This showed that interesting spin phenomenon can be realized in materials without the need of large magnetic fields. The quantized version of the spin hall effect in an insulator (QSHE), which would provide chiral spin-polarized edge states, was proposed a year later involving a model of graphene with spin-orbit coupling (SOC),[17] however the SOC in graphene is too small to allow experimental observation of the predicted behavior of this material. An independent proposal for the QSHE by Bernevig, Hughes, and Zhang in 2006 in thin layers of HgTe/CdTe[18] and was

experimentally realized the following year by König et al.[19]

2 then, TIs have become an active research area in condensed matter from both theory and experiments. As this is a relatively new field, there is a rush to publish the ‘more exciting’ results leaving basic surface science questions largely unaddressed. This rapidly expanding field requires careful and diligent sample characterization because although its quantum phenomena are guaranteed by its invariant, real world conditions can complicate the study of the interesting TI physics. The new results of this thesis are largely focused upon identifying surface phenomena that interfere with access to TI physics. These include unusual surface termination (Chapter 3), bulk dopant segregation (Chapter 4), and topologically trivial adsorbate-induced interface states (Chapter 5).

In the present Chapter, a brief background in solid states physics is provided focusing on the concepts of a crystalline solid and its electronic structure that are most relevant to TI studies. This is followed by an introduction to the topological band theory of solids where the Z2 topological invariant, time-reversal symmetry, and TI properties are discussed. Next, a historical perspective of experimental evidence for 3D TIs is given for context on the approaches used for controlling and modifying the properties of TIs. This leads into a section highlighting the current materials science challenges for synthesis and characterization of these materials. A section on molecular orbital (MO) theory is provided illustrating the advantages of using organic molecules as an alternative approach to controlling and modifying TIs. Finally, an overview of the literature of the experimental results of organic-TI interfaces is discussed.

**1.2 Crystallography Background **

Crystallography was celebrated worldwide in 2014 as the International Year of Crystallography being recognized by the United Nations for, “its importance in our understanding of the material nature of the world”. The atomic building blocks of our universe are of course too small to be imaged optically but can be detected by diffracting high energy photons from a periodic array of atoms revealing their physical structure. This thesis consists of primarily of experimental studies of single crystals and a background of physics of solid states will be of use.

We begin by considering a general periodic array of atoms in 3D which consists of all points with positions vectors of the form

𝐑 = 𝑛1𝒂1+ 𝑛2𝒂𝟐+ 𝑛3𝒂3 1.1

3 and is often chosen to describe the crystal structure. The diffraction of light in these crystallographic materials rely on photons interfering constructively directly probing its periodicity.

The reciprocal lattice is a fundamental concept in condensed matter and is defined to be a dual vector space to the real space lattice using the basis vectors:

𝐛1= 2𝜋

𝐚2× 𝐚3 𝐚1∙ (𝐚2× 𝐚3)

1.2

𝐛2 = 2𝜋

𝐚3× 𝐚1 𝐚1∙ (𝐚2× 𝐚3)

1.3

𝐛3 = 2𝜋

𝐚1× 𝐚2 𝐚1∙ (𝐚2× 𝐚3)

1.4

The reciprocal lattice can then be described by the set of all wave vectors, where ki are integers

𝐊 = 𝑘1𝐛1+ 𝑘2𝐛2+ 𝑘3𝐛3 1.5

The first Brillouin zone (BZ) is the Wigner-Seitz primitive cell of the reciprocal lattice and while they refer to identical geometries the former is typically used in the condensed matter community. Since real materials are made up of some Avogadro’s number of atoms the consideration of this system as infinite is justified, although it is important to examine the effects of the boundaries (i.e. surfaces). The plane of the BZ that defines the surface is indicated by its miller indices (hkl) corresponding to a plane normal to the reciprocal lattice vector hb1 + kb2 + lb3. It is important to note that complete knowledge of all observables of the electrons (e.g. dispersion) is contained within this unit cell.

The electronic structure of these crystalline solids can be approximated with an independent
electron model considering a one-electron potential (U(**r**)). The electrons that are solutions to the
Schrodinger equation with a periodic potential are referred to as Bloch electrons. These allowed
electronic states form energy bands which is Bloch band theory. The next section shows how this
approximation can be used to obtain the electronic band structure of solids.

4
The Schrodinger equation for the one-electron Hamiltonian, ℋ, with a periodic potential U(**r **+

**R**)=U(**r)** is:

ℋ𝜓 = (− ℏ 2

2𝑚∇

2_{+ U(𝐫)) ψ = Eψ } _{1.6}

The Bloch wavefunction satisfies the Schrodinger equation for a periodic potential which gives a good approximation for the states of an electron in single crystals.[21]

ψ(𝐫 + 𝐑) = 𝑒𝑖𝐤∙𝐫ψ(𝐫) 1.7

Bands of allowed states are formed in solid crystalline materials where their energetic position in reciprocal space (henceforth k-space) depend on the crystals symmetry and chemical properties.

Conductors have overlapping conduction and valence bands whereas insulators, which include semiconductors, have a gap in these bands.

The tight-binding model begins by considering a localized wave function at each atomic site in a
lattice. In the single-particle view, first suppose we have a 1D lattice of N atoms separated by a distance,
*a. We can write the Bloch wave function as: *

|Ψ > = 1 √N∑ 𝑒

𝑖𝒌∙𝐑

𝑹

|Φs(𝐫 − 𝐑) > 1.8

where the atomic positions are labelled by R and only an s-orbital basis Φs is being considered. The goal is to solve the time-independent Schrodinger equation (ℋ|Ψ > = E|Ψ >) considering only summing over nearest-neighbors and ignoring direct overlap (< Φs|Φs(𝒓 − 𝑹) > = 0). To do this, we project the s-orbital as follows:

< Φs|ℋ|Ψ > = E < Φs|Ψ > 1.9

where the wave function is

|Ψ > = 1

√N(|Φs> + 𝑒
𝑖𝑘𝑎_{|Φ}

s(𝑟 − 𝑎) > + 𝑒−𝑖𝑘𝑎|Φs(𝑟 + 𝑎) >) 1.10

5

< Φs(𝐫)|ℋ|Ψ > = 1

√N ( < Φs|ℋ|Φs> + 𝑒

𝑖𝑘𝑎_{< Φ}

s|ℋ|Φs(𝑟 − 𝑎) > +

𝑒−𝑖𝑘𝑎_{< Φ}

s|ℋ|Φs(𝑟 + 𝑎) >) 1.11

This reduces to

< Φs(𝐫)|ℋ|Ψ > = 1

√N(E𝑠+ 𝑡𝑒

𝑖𝑘𝑎_{+ 𝑡𝑒}−𝑖𝑘𝑎_{)} _{1.12}

where E*s* is the energy of the s-orbital and t is the hopping term which characterizes the tunneling of an
electron from one site to its nearest-neighbor. The right hand side of Equation 1.9 is:

E < Φs|Ψ >= 1

√N(E < Φs|Φs> +E 𝑒

𝑖𝑘𝑎_{< Φ}

s|Φs(𝑟 − 𝑎) > +E𝑒−𝑖𝑘𝑎< Φs|Φs(𝑟 + 𝑎) >) 1.13

The last two terms are equal to zero and then is reduced to

E < Φs|Ψ ≥ 1

√NE 1.14

And putting the left and right hand side back together

1

√N(Es+ 𝑡𝑒

𝑖𝑘𝑎_{+ 𝑡𝑒}−𝑖𝑘𝑎_{) =} 1

√NE 1.15

And finally solving for E we get

E = Es− 2𝑡𝑐𝑜𝑠(𝑘𝑎) 1.16

This is showing the dispersion relation, E(k), and the allowed energy states that make up the band structure in a crystal. While this is only a 1D model with a single band, it qualitatively shows how a tight-binding approach can be used to elucidate the band structure of a material.

6 The insulating state of crystalline solids has a chemical potential which falls in the electronic energy gap of the bulk Bloch bands. We know that a semiconductor also has a band gap, and therefore can be regarded as an insulator and so the question arises; Are all insulators fundamentally the same? The answer is surprisingly no, and the fundamental property that distinguishes these states of matter is the topology of the band structure.

The IQHE is an insulator with a nontrivial topology, in which electrons with quantized Landau levels drift with cyclotron orbit frequency under an applied field. It was realized by Thouless, Kohmoto, Nightingale, and den Nijs (TKNN) that the IQHE is topologically nontrivial and they showed that in this system the k-space cane be mapped to a nontrivial Hilbert space and its topology can be specified by an interger topological invairaint. The connection of this 2D TI and the 3D TI is through the Chern invariant and can be physically understood in terms of the Berry phase.[4, 5, 22] It is imperative to emphasis that the topological Z2 invariant from 2D to 3D is a nontrivial generalization. Physically this can be

understood by noting that by stacking 2D TIs vertically does not guarantee chiral edge states on the top and bottom surfaces. Therefore, these are unique phases of matter but have important parallels and the pedagogical account provides context for the recent rapid development in the TI field.

The Berry phase is a modification to the wave-function distinct from its dynamical phase. To see this, consider the Bloch Hamiltonian:

ℋ|𝜓𝑛𝐤 >= 𝐸𝑛𝐤|𝜓𝑛𝐤> 1.17

for the nth eigenstate ψ at position k. The Bloch theorem allows this to be written as a plane wave times a function with the same periodicity of Bravais lattice:

𝜓𝑛𝐤(𝐫) = 𝑒𝑖𝐤∙𝐫𝑢𝑛𝐤(𝐫) 1.18

where u* nk*(

**r + R**) = u

*(*

**nk****r**) for all

**R**in the Bravais lattice. The Berry connection, 𝒜

_{𝑛}, is given by:

𝒜𝑛 = 𝑖 < 𝜓𝑛𝒌|∇𝑘|𝜓𝑛𝒌> 1.19

quantum-7 mechanical system accumulates a phase factor after completing a closed path in k-space. The curl of the Berry connection defined as the Berry curvature, 𝓕𝒎:

𝓕𝒎 = 𝛁𝒎 x 𝒜𝑚 1.20

and the TKNN invariant, also called the Chern number, is the integral of the Berry curvature over the Brillouin zone:

𝒏𝒎 = 1 2𝜋∫ 𝑑

2_{𝐤 𝓕}

𝒎 1.21

That is, it is equal to the Berry phase of the Bloch wavefunction calculated around the Brillouin zone
boundary divided by 2π. The total Chern number summed over all the contribution from the nth band, n*m*
is equal to n:

𝑛 = ∑ 𝑛𝑚 𝑁

𝑚=1

1.22

is connected to the Hall conductivity such that σxy=Ne2_{/h, where n =N. This tells us that the quantum Hall }
state is a TRS-breaking system an is often referred to as a Chern insulator. The quantum spin Hall state is
the spin version of the IQHE and can be thought of as two copies of the quantum Hall system with
spin-polarized chiral edge states, recovering the TRS of the system.[4] Kane and Mele showed that the
topological invariant for TRS systems can be characterized by a Z2 index[23] which is formulated below.

A TRS system is can be described by first introducing the time-reversal operator which is antiunitary and its form is given below:

### Θ = 𝑒

(𝑖𝜋𝑆ћ𝑖)_{𝐾,}

_{where Θ}

2_{ = −1}

_{1.23}

8

### Θℋ(𝐤)Θ

−1### = ℋ(−𝐤)

1.24where **k** represent Bloch wave vectors. The Bloch energy bands are then degenerate at the time-reversal
invariant momentum (TRIM) in the BZ and are referred to as Kramers pairs.[4] In a 2D BZ there are 4
TRIMs and for the 3D BZ there are 8 TRIMs.[24] To formulate the Z2 topological invariant and its
connection to the Berry phase, a unitary matrix is defined:

### 𝑤

_{𝑚𝑛}(

### 𝐤

)### =< 𝑢

_{𝑚,−𝐤}

### |Θ|𝑢

_{𝑛,𝐤}

### >

1.25where m, n indicate the quantum numbers and **k** is the momentum quantum number for the respective
eigenstates. The Bloch states are then related by:

|𝑢𝑚,𝐤 > = ∑

### 𝑤

𝑚𝑛∗ (𝐤)Θ|𝑢𝑛,𝐤> 𝑛1.26

The unitary matrix has the following relation:

### 𝑤

𝑛𝑚(−𝐤) = −𝑤𝑚𝑛(𝐤) 1.27which means that it becomes antisymmetric at a TRIM Λ. For a skew-symmetric matrix, the square of a
polynomial can be written for its matrix entries. The value of the polynomial applied to the coefficients of
the matrix is called the pfaffian. In general, the determinant of an antisymmetric matrix is equal to the
square of its Pfaffian (Pf(A)2_{ = det(A))[4, 5] }

𝛿𝑎=

𝑃𝑓[𝑤(Λ𝑎)] √𝐷𝑒𝑡[𝑤(Λ𝑎)]

= ±1 1.28

The Z2 invariant, ν, for a 2D system is then:

(−1)𝜐_{= ∏ 𝛿}
𝑎
4

𝑎=1

1.29

9

𝑁𝐾= Δ𝜐 mod 2 1.30

The topological invariant Z2 index can be thought of as the number of times an edge states crosses the Fermi level between 0 and π/a as even or odd, where a is the crystal’s lattice constant.[4] The Z2 invariant in a 3D crystal with inversion symmetry has parity eigenstates with eigenvalues ξm(Λa) = ± 1and is then:

𝛿𝑎= ∏ 𝜉𝑚(Λ𝑎) 𝑚

1.31

The ingredients for a TI are now given by a bulk insulating material that has an odd number of inversions at the TRIM. The topological invariant must change at the boundary of a trivial and nontrivial insulator resulting in the closing of the energy gap.

Surface states can arise when the potential barrier formed at the crystal termination is such that an allowed state exists which decays exponentially away from the surface as shown by Shockley.[25] These states are confined only to the surface and they are often referred to as a 2D electron-gas (2DEG). The atomic layer at the termination of the crystal has some electron density above the surface and the near surface charges will arrange such that an electric dipole is formed at the surface. When a strong SOC is present at the surface,

ℋ̂SOC∝ (𝐄 × 𝐩) ∙ 𝛔 1.32

10 Until 2015, the Rashba split surface states of Au(111) were thought to be topologically distinct from the TSS, often being described as a clear example of a topologically trivial surface state. This is now being disputed as theoretical and experimental investigations have claimed these states to be topologically derived surface states again demonstrating the very fast pace of this field.[26] The often quoted

distinction relied on the TSS being linearly dispersing, at least near the Dirac point, and these new results indicate that the warping term is strong enough to distort the dispersion. This occurs in Bi2Te3 away from the Dirac point where the Fermi surface evolves from a cone-like to snowflake-like due to the strength of the λ SOC term. The surface BZ of TIs studied in this thesis is shown in Figure 1.2 with the symmetry points labelled and a circle with arrows indicating the spin texture of the TSS which also illustrate the forbidden backscattering in absence of a spin-flip mechanism.

11

**1.5 Model Hamiltonian for Binary TIs **

The theoretical development for TR invariant systems characterized by a Z2 topological index used the tight-binding model for graphene with strong spin-orbit coupling. This model includes the π-orbitals of the honeycomb carbon atoms near K and K’ in the hexagonal BZ, considers the symmetry of the lattice, and includes spin with TRS spin-orbit interactions. Kane and Mele predicted that for a finite SOC the material would become a quantum spin hall insulator, however the intrinsic SOC is very weak and difficult to observe experimentally. An independent proposal by Berneving, Hughes, and Zhang (BHZ model) considered the s- and p-orbitals of HgTe with a cubic zinc-blende crystal structure lead to the first experimental discovery of the first 2D TI.

The band structure of the binary chalcogenide 3D TIs, Bi2Te3 and Bi2Se3, was examined in detail by Liu et al. and derived the model Hamiltonian for these systems in a few ways.[1] The important symmetry for these 3D TIs, in addition to TRS, is inversion symmetry. The unit cell has two equivalent Bi atoms and two equivalent Se or Te atoms and one inequivalent Se or Te atom where the inversion occurs. Only the p-orbitals are considered for in their band structure calculation as these are the outermost electron shells. The bonding within the unit cell is of covalent nature and is stronger than the van der Waals force that holds the layers together. I will outline the inversion of the Bi and Te/Se bands following the symmetry arguments in Section II from Lui et al.

The Bi atomic p-orbitals are higher in energy than the Se/Te atomic p-orbitals and then

considering the bonds formed within a QL, the hybridized Bi states are pushed up while the Se states are

**Figure 1.2** (a) Schematic of the bulk bands and TSS showing the forbidden backscattering
where an electron at k*i* must flip its spin to transition to -k*i*. (b) The hexagonal surface BZ of
the strong 3D TIs studied in this thesis with symmetry points indicated. The purple circle
represents Fermi surface of the Dirac cone with spin locked perpendicular to its

12
pushed down. Since the inversion center Se/Te atom forms a bond with both Bi atoms, it is more stable
and therefore lower in energy and no longer being considered. The new states consist of bonding and
antibonding orbitals and it is convenient to write these orbitals in terms of a definitive parity. The parity
operation flips the sign of one spatial coordinate and the parity operator is P. This can be seen by
considering a π-bond formed by two pz orbitals making bonding states, |𝜋 > (see Figure 1.6 (c)) have a
parity of -1 and antibonding states, |𝜋∗_{>}_{ , have parity +1. That is }

𝐏|π > = −|π > 1.33

𝐏|𝜋∗> = +|𝜋∗> 1.34

The bonding and antibonding states are written as a liner combination of the equivalent atomic orbitals so that 4 new states are formed. The bonding states of Bi are pushed down while the antibonding states of Se/Te are pushed up towards the Fermi level. As the crystal structure is layered, the pz orbitals have a different interaction than the px and py orbitals, and they are pushed toward the Fermi level. That is, before taking SOC into account, the conduction band mainly consists of Bi pz orbitals while the valence band mainly consists of Se pz orbitals. The SOC couples the pz orbitals to a linear combination of px and py orbitals, and when strong enough will induce a level crossing of states of opposite parity. So, the inversion of these states of mixed atomic-orbitals and opposite parity at a time-reversal invariant momenta distinguishes these materials as topologically nontrivial insulators.

Note that the inversion occurs only at a single point in the BZ and so, considering only a single band, will have positive parity and negative parity at various points in the BZ. Because the parity

eigenvalues are discrete, there cannot be a smooth transformation from one eigenvalue to the other. In this sense the bulk bands are of mixed character and are a hybridization of conduction and valence bands. Additionally, it is important to note here that insulating is defined as an energy gap between conduction and valence bands at every point in the BZ and does not necessarily mean the material will be electrically insulating. In fact, a major materials science challenge is to be able to synthesize crystals with very low bulk free carriers.

The low-energy effective Hamiltonian for the binary TIs in the bulk was derived by Liu et al.[1] by symmetry principles and 𝒌 ∙ 𝒑 pertrubation theory. It is a four band model that effectively describes the behavior of the conduction and valence bands near the Gamma-point.

ℋ(𝒌) = 𝜖0⊥(𝐤)I4×4+ (

𝑀(𝐤) 𝐴1k𝑧 0 𝐴2k− 𝐴1k𝑧 −𝑀(𝐤) 𝐴2k− 0

0 𝐴2k+ 𝑀(𝐤) −𝐴1k𝑧 𝐴2k+ 0 −𝐴1k𝑧 −𝑀(𝐤)

13
where 𝑘±= 𝑘𝑥± 𝑖𝑘𝑦, 𝜖0(𝐤) = C + D1𝑘𝑧2 +D2𝑘⊥2, and M(**k**) = M – B1𝑘𝑧2 – B2𝑘⊥2. The coefficients used for
the band structure plots are given in table IV of Liu et al.[1]

The model Hamiltonian is written in the basis of |𝑃1−+, ± 1

2> and |𝑃2+
−_{, ±}1

2>, where |𝑃1−
+_{,}

±1 2> =

1

√2(|𝐵±1 2⁄ > ∓|𝐵_{±1 2}⁄

′ _{>)}_{ is the combination of bonding and antibonding orbitals for bismuth }
p-orbitals and |𝑃2+−, ±

1 2> =

1

√2(|𝑆±1 2⁄ > ∓ |𝑆±1 2⁄
′ _{>)}

is a combination of bonding and antibonding orbitals for selenium giving a definitive parity for each state. Diagonalizing the matrix gives the

eigenvalues and eigenvectors for these states and is shown in Figure 1.3. The order of the spin-degenerate
bands is inverted near **k**=0 while maintaining an energy gap which characterizes the nontrivial topology
of these materials.

The topological surface states are obtained by diagonalizing the Hamiltonian in Equation 1.35 with an open boundary condition resulting in the following surface Hamiltonian[1, 20]

14

ℋ(𝒌) = E0(𝑘) + 𝑣𝑘(𝑘𝑥𝜎𝑦− 𝑘𝑦𝜎𝑥) + 𝜆 2(𝑘+

3_{+ 𝑘}

_3)𝜎𝑧 1.36

where E0(𝑘) is the energetic position of the Dirac point, 𝑘±= 𝑘𝑥± 𝑖𝑘𝑦, vk is the Fermi velocity, and λ is a SOC warping parameter. The solution then gives the surface band dispersion relation:

E±(𝒌) = E0(𝑘) ± √𝑣𝑘2𝑘2+ 𝜆2𝑘6cos6(3θ) 1.37

where ± represent the unoccupied and occupied bands which touch at the Dirac point. The topological
surface states are spin-chiral and gapless as a result of applying these boundary conditions (illustrated in
Figure 1.2). Notice that the energy of the Dirac fermions is proportional to their velocity, i.e. linear
dispersion, in contrast to the 2DEG which disperses quadratically (E(k) ∝ v2_{). }

The dispersion of the surface states can be directly measured by photoelectron spectroscopy and scanning tunneling microscopy as described in the next Chapter and the next section overviews the use of these experimental techniques in the discovery of 3D TIs.

**1.6 Experimental Evidence for 3D Topological Insulators **

What experimental evidence is necessary in order to determine that a material is indeed a TI? This requires a surface sensitive technique to determine the existence of a TSS and that the material is bulk-insulating. The instrumental workhorse for probing TIs has been angle-resolved photoemission spectroscopy (ARPES) which maps photoemitted electrons energy to their position in k-space (see Chp. 2). Spin-resolved data is necessary to determine that the TSS electron’s spin is locked perpendicularly to their momenta. As will be discussed below, synthesis of TIs has a materials science challenge of reducing charge carriers, and only it is only when the sample is sufficiently insulating with high surface carrier mobility that a material can be confirmed as a TI through transport. To do so it must be shown that the sample has transport occurring through the surface and that the carriers are indeed Dirac fermions. These are completed through sample-size dependence on conductance and determining the π Berry phase from quantum oscillations.[19, 27]

Experimental proof of a strong 3D TI was first achieved using photoelectron spectroscopy to map the 2D topological surface state in the alloy Bi1-xSbx.[28] Bismuth is a semimetal which is where the BCB and BVB touch, with topologically trivial surface states. When Antimony is substituted in at

15 resulting in a quantum phase transition to a nontrivial insulator and consequently, a nontrivial surface state appears in addition to the trivial surface states of Bi. To prove it’s a strong 3D TI, resistivity as function of temperature for Sb concentrations of x=0 and x =0.1 is presented showing the semimetallic and insulating character, respectively. The topological nature of the surface state was determined by ARPES mapping the near Ef photoemitted electrons at the TRIM which showed a Kramers degenerate point. The TSS was further supported by varying the incident photon energy which allows probing in the direction perpendicular to the surface and found that this feature does not disperse (i.e. it’s a surface state). These measurements are consistent with a strong 3D TI and was quickly confirmed when spin-resolved ARPES provided the first direct evidence of a π Berry phase by showing the spin polarization indeed rotates by 360˚ around the Fermi surface.[29]

The complex surface state structure of Bi1-xSbx make this material an unsuitable candidate for detailed studies of the interesting physics associated with the TSS as it coexists with trivial surface states. TIs with a single TSS were predicted by Zhang et al. in the binary class of binary materials Bi2Se3, Bi2Te3, and Sb2Te3, the same year proposing a low-energy effective Hamiltonian model to describe the bulk band structure.[1] Experimental photoelectron spectroscopy studies of these materials quickly confirmed them to be strong 3D TIs. These quickly became the prototypical TIs as the synthesis of binary phases of materials is simpler in principal and can produce higher purity samples. The Z2 topological invariant is (1;000) which supports a single TSS centered at the Γ point of the surface BZ which ideally provides a simple topological Dirac cone to experimentally probe. However, in practice there are inherent challenges in accessing the TSS in each of these systems which will be addressed below.

**1.7 Breaking Time-Reversal Symmetry **

The Z2 topological invariant in strong 3D TIs guarantees a gapless surface state unless TRS is broken. Ferromagnetic ordering mediated by the surface Dirac electrons has been proposed theoretically to break TRS where the exchange coupling of the Dirac electron spin, σ, and the localized spin of the magnetic impurity, S, are modeled by the Hamiltonian:

ℋ = ℏ𝑣(𝐤 × 𝒛̂) ∙ σ − 𝐽𝑛0𝑆𝑧σ𝑧 1.38

16 When TRS is broken, a gap opens in the TSS resulting in the quantum anomalous hall effect (QAHE), that is a quantized Hall effect without an external magnetic field.[30] The surface state dispersion can then be written:

E±(𝑘) = ED± √(ℏ𝑣)2𝑘2+ ∆2 1.39

where ED is the energy of the Dirac point and Δ= 𝐽𝑛0𝑆𝑧σ𝑧/2 is the size of the magnetically induced Dirac-mass gap.[31]

The approaches to breaking TRS have been to bulk-dope the TI during the synthesis process and more recently organic molecules have been used.[32-37] Bulk-doping with magnetic impurities may be a suitable route for this magnetic dopant approach as ferromagnetic ordering with perpendicular magnetic anisotropies has been achieved.[38, 39] However, because the TSS exists at the surface it may be more advantageous to use magnetic organic molecules deposited on the surface to elucidate the interaction of the TSS with a magnetic impurity.[40]

The nature of topology in condensed matter can then be investigated as it is TRS that guarantees the existence of a TSS. Understanding how magnetic dopants interact with the TSS is important. An indication of breaking TRS is a gap opening in the TSS as the spin degeneracy at the Dirac point is lifted. The opening of a gap in the TSS has been also been studied by ARPES and has been found in TIs that lack the out of plane ferromagnetism required to break TRS, possible caused by impurity-induced

resonance states.[41] Transport measurements have possibly observed the quantum anomalous Hall effect in magnetically doped TIs although at the very low temperature of ~30 mK.[42] Thus, there are a lot of opportunities to investigate this symmetry breaking in these systems, particularly in the choice of magnetic impurity, as well as understanding the impact of nonmagnetic impurities in the formation of a gapped surface state.

**1.8 Surface Science Challenges for TI Research **

17 are present as strong band bending at the surface of Bi2Se3 has been shown to create a coexisting 2-DEG with the TSS.[43] Furthermore, it is expected that cleaving this material would result in a Se-terminated surface, as these are the layers that are bound by the weaker vdW forces. However, as will be shown in Chapter 3, cleaving Bi2Se3 can result in coexisting Bi- and Se-terminated which strongly modifies the valence band structure.[46]

Bi2Te3 alleviates some of the synthesis issues, as it can be grown in both n- and p-type by varying the composition concentration of the initial growth, however the carrier density is still difficult to reduce. Additionally, the Dirac point is below the top of the M-shaped valence band. This presents an

experimental challenge in accessing the interesting physics of the TSS as, for example, scattering vectors between the TSS and BVB are available making quasiparticle interference analysis challenging.

Additionally, due to strong SOC from the Te, the TSS becomes warped from conical to a snowflake-like shape away from the Dirac point. Contrarily, the TSS of Bi2Se3 is conical far away from the Dirac point and above the BVB maximum which is ideal to probe the TSS. However, as mentioned earlier this material is difficult to synthesize as an insulator.

18 Bulk-doping has been the typical approach used to modify the properties of TIs where dopants may be substituted at a lattice point or intercalate between the QLs. As is shown in Chapter 4, issues of phase-segregation can complicate the synthesis process. This is illustrative of some of the basic materials science challenges that have yet to be addressed in this new and exciting field. The next section outlines an alternative approach which is to use organic molecules.

**1.9 Molecular Orbital Theory **

Organic molecules are another avenue for controlling and modifying the properties of TIs and is a term which generally applies to hydrocarbon based molecules. One advantage to this approach is the chemical tunability offered by modifying some molecule constituent changing its physical properties. The phthalocyanine molecule is a dye used in commercial applications and one of the most studied molecules for its optical, electronic, and magnetic properties.[47, 48] It is a planar molecule consisting of aromatic macrocycles and substitution of a central transition-metal atom allows for tuning of its electronic and magnetic properties. In this section molecular orbital theory will be used to understand the properties of MPcs.

19 Bonding of atoms in molecules consists of an overlap of electron densities and it is useful to recall the symmetry of the atomic orbitals. For instance, consider a p-orbital which has a lobe pointed towards an s-orbital. This has a symmetry that allows for the orbitals to overlap which results in a σ bond, however if the p- and s-orbital are arranged as in Figure 1.5 (b), then they will have no overlap and not result in a bond forming.. A π-bond is formed by two pz-orbitals (Figure 1.5 (c)), for example, that have both of their lobes overlapping. The valence electrons in Carbon occupy the p-orbitals and allow for a hybridization of C p-orbitals resulting in delocalized electrons referred to as a π-electron cloud. This is one of the many reasons organics have received a lot of attention for electronic devices.

Ligand-field theory is a useful tool for describing how the symmetry of a transition metal compound splits these energetically degenerate atomic orbitals and arrange into molecular orbitals.[49] Essentially the theory uses the molecules symmetry to classify it to a point group specifying the possible linear combination of atomic orbitals (LCAO). So by knowing the symmetry of the molecule, the ordering of its bonding and antibonding MOs can be elucidated. It is noted that this is a qualitative description and the ordering needs to be verified by experiments.

20 The MPc molecule has a central transition-metal with valence electrons in its d-orbitals that split

according to its D4h point group. In ligand-field theory the principal axis is determined by the axis with the highest symmetry, which is four-fold in this case. The D denotes the dihedral group which contain two n-fold axes perpendicular to the principal axis. The h denotes a horizontal mirror plane that exists perpendicular to the principle plane. The rotations and mirror planes for this point group are shown in Figure 1.7 overlaid on the MPc molecule. Character tables for each point group can be easily looked up and show the allowed symmetries and ordering of molecular orbitals.

21 The d-shell for the D4h point group are arranged as shown in Figure 1.8 and the occupation is shown for the MnPc molecule. Filling of the d-shell occurs as the 3d transition-metal increases in atomic number changing the properties of MPc molecule. Magnetism in thin films of the half-filled d-shell MPcs has been reported and single molecules can be thought of as molecular magnets.[48] Single molecules are of course paramagnetic as no preferential ordering occurs whereas in thin films ferromagnetic ordering can occur. The rich physics of the MPc molecules can be appreciated from an applied side, for example in the case of CuPc and organic photovoltaics, as well as from a fundamental perspective in the case of studying the Kondo effect. Systematic study of the 3transition-metal Pc molecules have identified the role of d-shell filling as well as the isoindole ligands in its adsorption, electronic, and magnetic properties. These molecules offer a playground to investigate the relatively new field of organic-TI interfaces. In particular, the random distribution of magnetic atoms in bulk-doping can be eliminated as complete monolayers of an MPc can be grown.

**1.10 Survey of Organic-TI interface **

**Figure 1.7** The D4h symmetry elements for the MPc molecule are shown. The highest

22 The first experimental study of the organic-TI system was performed on the electron acceptor molecule F4-TCNQ on the degenerately n-doped Bi2Se3. Kim et al. showed the fundamental signature of the TSS in ambipolar electron transport on the surface of a bulk insulating film for the first time.[50] This established small organic molecules in the TI field as a tunable knob for controlling bulk doping. Our group further investigated this system by characterizing the charge transfer, work function shift, and growth morphology of F4-TCNQ on Bi2Se3 TI samples grown by binary melt and hybrid physical-chemical vapor deposition.[51] This molecule and the unflorinated TCNQ have also recently been shown to tune the carrier density of BSTS and convert it to a p- or n-type semiconductor. It is therefore clear that electronic-doping TIs via organic molecules is a nondestructive approach for controlling carrier types.[52]

Molecules can also be used as an approach to breaking TRS in TI systems. The first studies of
MPcs on TIs were performed by STM groups on the system MnPc/ Bi2Te3[53] and FePc/Bi2Te3[37] in
2014. Since then, there have been a handful of experimental studies of the MPc-TI interface with general
agreements that the TSS remains unperturbed by the organic molecules.[54-56] Differences in monolayer
growth and charge-transfer effects have been observed that depend on the d-shell filling where the
spatially extended dz2_{ orbital lies close to the Fermi level for the lower atomic numbers.[57] }

The organic-TI studies thus far have led to interesting observations such as protection of the TSS and hybrid-interface states forming (HIS), and even theoretical predictions for a 2D organic TI in a

23 organic framework.[56, 58, 59] Careful analysis of quasiparticle interference data is needed to understand the scattering potential associated with an adsorbed magnetic molecule. In particular, spin-resolved measurements are likely needed to elucidate the interactions of a magnetic potential on the TSS.[60]

The next chapter will review the analytical instruments and experimental methods that were used followed by presentation of three selected studies:

In Chapter 3 a photoemission spectroscopy study on the surface termination of the TI Bi2Se3 is presented. It is shown that the environment in which the crystal is cleaved has a mechanical effect resulting in different terminated surface which strongly modifies the valence band electronic structure. This work has been published in the Journal of Vacuum Science and Technology B.

Chapter 4 presents a photoemission study of Cr-doping the topological insulator BSTS as a route to breaking TRS. It is shown that for high concentrations of Cr, impurity phases are formed during the synthesis suggesting an alternative route to break TRS in TIs.

Chapter 5 presents a systematic study of the organic molecule MnPc adsorbed on Bi2Te3 showing a previously unobserved hybrid-interface state (HIS). Photoelectron spectroscopy shows charge transfer occurring and the HIS forming

**References **

1. Liu, C.-X., et al., Model Hamiltonian for topological insulators. Physical Review B, 2010. **82**(4):
p. 045122.

2. Fert, A., Nobel Lecture: Origin, development, and future of spintronics*. Reviews of Modern
Physics, 2008. **80**(4): p. 1517-1530.

3. Brumboiu, I.E., et al., Elucidating the 3d Electronic Configuration in Manganese
*Phthalocyanine. The Journal of Physical Chemistry A, 2014. ***118**(5): p. 927-932.

4. Ando, Y., Topological Insulator Materials. Journal of the Physical Society of Japan, 2013.

**82**(10): p. 102001.

24
6. Pan, Z.H., et al., Measurement of an Exceptionally Weak Electron-Phonon Coupling on the
*Surface of the Topological Insulator ${\mathrm{Bi}}_{2}{\mathrm{Se}}_{3}$ Using Angle-Resolved *
*Photoemission Spectroscopy. Physical Review Letters, 2012. ***108**(18): p. 187001.

7. Yang, F., et al., Dual-Gated Topological Insulator Thin-Film Device for Efficient Fermi-Level
*Tuning. ACS Nano, 2015. ***9**(4): p. 4050-4055.

8. Rojas-Sánchez, J.C., et al., Spin to Charge Conversion at Room Temperature by Spin Pumping
*into a New Type of Topological Insulator: $\ensuremath{\alpha}$-Sn Films. Physical Review Letters, *
2016. **116**(9): p. 096602.

9. Yuan, J.-H., et al., The spin polarization and transport properties at the surface of a
*three-dimensional topological insulator. Solid State Communications, 2015. ***206**: p. 31-37.

10. Fan, Y., et al., Electric-field control of spin–orbit torque in a magnetically doped topological
*insulator. Nat Nano, 2016. ***11**(4): p. 352-359.

11. Li, H. and A. Manchon, Tunable spin-charge conversion through topological phase transitions in
*zigzag nanoribbons. Physical Review B, 2016. ***93**(23): p. 235317.

12. Hasan, M.Z. and J.E. Moore, Three-Dimensional Topological Insulators. Annual Review of
Condensed Matter Physics, 2011. **2**(1): p. 55-78.

13. Alicea, J., et al., Non-Abelian statistics and topological quantum information processing in 1D
*wire networks. Nat Phys, 2011. ***7**(5): p. 412-417.

14. Klitzing, K.v., G. Dorda, and M. Pepper, New Method for High-Accuracy Determination of the
*Fine-Structure Constant Based on Quantized Hall Resistance. Physical Review Letters, 1980. ***45**(6): p.
494-497.

15. von Klitzing, K., Developments in the quantum Hall effect. Philosophical Transactions of the
Royal Society of London A: Mathematical, Physical and Engineering Sciences, 2005. **363**(1834): p.
2203-2219.

16. Kato, Y.K., et al., Observation of the Spin Hall Effect in Semiconductors. Science, 2004.

**306**(5703): p. 1910-1913.

17. Kane, C.L. and E.J. Mele, Quantum Spin Hall Effect in Graphene. Physical Review Letters, 2005.

**95**(22): p. 226801.

18. Bernevig, B.A., T.L. Hughes, and S.-C. Zhang, Quantum Spin Hall Effect and Topological Phase
*Transition in HgTe Quantum Wells. Science, 2006. ***314**(5806): p. 1757-1761.

19. König, M., et al., Quantum Spin Hall Insulator State in HgTe Quantum Wells. Science, 2007.

**318**(5851): p. 766-770.

25 21. Bloch, F., Über die Quantenmechanik der Elektronen in Kristallgittern. Zeitschrift für Physik.

**52**(7): p. 555-600.

22. Thouless, D.J., et al., Quantized Hall Conductance in a Two-Dimensional Periodic Potential.
Physical Review Letters, 1982. **49**(6): p. 405-408.

23. Kane, C.L. and E.J. Mele, ${Z}_{2}$ Topological Order and the Quantum Spin Hall Effect.
Physical Review Letters, 2005. **95**(14): p. 146802.

24. Fu, L., C.L. Kane, and E.J. Mele, Topological Insulators in Three Dimensions. Physical Review
Letters, 2007. **98**(10): p. 106803.

25. Shockley, W., On the Surface States Associated with a Periodic Potential. Physical Review,
1939. **56**(4): p. 317-323.

26. Manchon, A., et al., New perspectives for Rashba spin-orbit coupling. Nat Mater, 2015. **14**(9): p.
871-882.

27. Brune, C., et al., Spin polarization of the quantum spin Hall edge states. Nat Phys, 2012. **8**(6): p.
485-490.

28. Hsieh, D., et al., A topological Dirac insulator in a quantum spin Hall phase. Nature, 2008.

**452**(7190): p. 970-974.

29. Hsieh, D., et al., Observation of Unconventional Quantum Spin Textures in Topological
*Insulators. Science, 2009. ***323**(5916): p. 919-922.

30. Yu, R., et al., Quantized Anomalous Hall Effect in Magnetic Topological Insulators. Science,
2010. **329**(5987): p. 61-64.

31. Lee, I., et al., Imaging Dirac-mass disorder from magnetic dopant atoms in the ferromagnetic
*topological insulator Crx(Bi0.1Sb0.9)2-xTe3. Proceedings of the National Academy of Sciences, 2015. *

**112**(5): p. 1316-1321.

32. Chen, Y.L., et al., Massive Dirac Fermion on the Surface of a Magnetically Doped Topological
*Insulator. Science, 2010. ***329**(5992): p. 659-662.

33. Wray, L.A., et al., A topological insulator surface under strong Coulomb, magnetic and disorder
*perturbations. Nat Phys, 2011. ***7**(1): p. 32-37.

34. Hor, Y.S., et al., Development of ferromagnetism in the doped topological insulator

*${\text{Bi}}_{2\ensuremath{-}x}{\text{Mn}}_{x}{\text{Te}}_{3}$. Physical Review B, 2010. ***81**(19): p.
195203.

35. Checkelsky, J.G., et al., Dirac-fermion-mediated ferromagnetism in a topological insulator. Nat
Phys, 2012. **8**(10): p. 729-733.

26
37. Song, Y.R., et al., Magnetic anisotropy of van der Waals absorbed iron(II) phthalocyanine layer
*on ${\mathrm{Bi}}_{2}{\mathrm{Te}}_{3}$. Physical Review B, 2014. ***90**(18): p. 180408.

38. Kulbachinskii, V.A., et al., Ferromagnetic transition in the new diluted magnetic semiconductor
*p-Bi2−xFexTe3. Physics Letters A, 2001. ***285**(3–4): p. 173-176.

39. Kulbachinskii, V.A., et al., Ferromagnetism in new diluted magnetic semiconductor
*Bi2−xFexTe3. Physica B: Condensed Matter, 2002. ***311**(3–4): p. 292-297.

40. Men'shov, V.N., et al., Magnetic proximity effect in the three-dimensional topological
*insulator/ferromagnetic insulator heterostructure. Physical Review B, 2013. ***88**(22): p. 224401.

41. Sanchez-Barriga, J., et al., Nonmagnetic band gap at the Dirac point of the magnetic topological
*insulator (Bi1-xMnx)2Se3. Nat Commun, 2016. ***7**.

42. Chang, C.-Z., et al., Experimental Observation of the Quantum Anomalous Hall Effect in a
*Magnetic Topological Insulator. Science, 2013. ***340**(6129): p. 167-170.

43. Bianchi, M., et al., Coexistence of the topological state and a two-dimensional electron gas on the
*surface of Bi2Se3. Nat Commun, 2010. ***1**: p. 128.

44. Analytis, J.G., et al., Bulk Fermi surface coexistence with Dirac surface state in

*${\text{Bi}}_{2}{\text{Se}}_{3}$: A comparison of photoemission and Shubnikov\char21{}de Haas *
*measurements. Physical Review B, 2010. ***81**(20): p. 205407.

45. Hor, Y.S., et al., $p$-type ${\text{Bi}}_{2}{\text{Se}}_{3}$ for topological insulator and
*low-temperature thermoelectric applications. Physical Review B, 2009. ***79**(19): p. 195208.

46. Hewitt, A.S., et al., Coexisting Bi and Se surface terminations of cleaved Bi2Se3 single crystals.
Journal of Vacuum Science & Technology B, 2014. **32**(4): p. 04E103.

47. Gottfried, J.M., Surface chemistry of porphyrins and phthalocyanines. Surface Science Reports,
2015. **70**(3): p. 259-379.

48. Bartolomé, J., C. Monton, and I.K. Schuller, Magnetism of Metal Phthalocyanines, in Molecular
*Magnets: Physics and Applications, J. Bartolomé, F. Luis, and F.J. Fernández, Editors. 2014, Springer *
Berlin Heidelberg: Berlin, Heidelberg. p. 221-245.

49. Griffith, J.S. and L.E. Orgel, Ligand-field theory. Quarterly Reviews, Chemical Society, 1957.

**11**(4): p. 381-393.

50. Kim, D., et al., Surface conduction of topological Dirac electrons in bulk insulating Bi2Se3. Nat
Phys, 2012. **8**(6): p. 459-463.

27
52. Tanabe, Y., et al., Electron and Hole Injection via Charge Transfer at the Topological Insulator
*Bi2–xSbxTe3–ySey–Organic Molecule Interface. The Journal of Physical Chemistry C, 2014. ***118**(7): p.
3533-3538.

53. Sessi, P., et al., Probing the Electronic Properties of Individual MnPc Molecules Coupled to
*Topological States. Nano Letters, 2014. ***14**(9): p. 5092-5096.

54. Bathon, T., et al., Systematics of Molecular Self-Assembled Networks at Topological Insulators
*Surfaces. Nano Letters, 2015. ***15**(4): p. 2442-2447.

55. Caputo, M., et al., Manipulating the topological interface by molecular adsorbates: Adsorption of
*Co-Phthalocyanine on Bi2Se3. Nano Letters, 2016. *

56. Yang, H.-H., et al., Organic Monolayer Protected Topological Surface State. Nano Letters, 2015.

**15**(10): p. 6896-6900.

57. Grobosch, M., et al., Engineering of the Energy Level Alignment at Organic Semiconductor
*Interfaces by Intramolecular Degrees of Freedom: Transition Metal Phthalocyanines. The Journal of *
Physical Chemistry C, 2009. **113**(30): p. 13219-13222.

58. Wang, Z.F., N. Su, and F. Liu, Prediction of a Two-Dimensional Organic Topological Insulator.
Nano Letters, 2013. **13**(6): p. 2842-2845.

59. Wang, Z.F., Z. Liu, and F. Liu, Organic topological insulators in organometallic lattices. Nat
Commun, 2013. **4**: p. 1471.

28

**CHAPTER 2 EXPERIMENTAL METHODS **

**2.1 Surface Science **

The surface of a crystal can host novel states of matter and experimentally we want to be sure that the surface is what we’re measuring. At the atomic level there are processes such as physiadsorption and phase transition and it is therefore necessary to diminish the number of these particles so that an isolated system can be used to perform experiments. A surface scientist only considers something to be clean once it’s been annealed in a vacuum.

This mantra does not excuse a messy room but is a key component to experiments. Our ambient environment is filled with particles that interfere with samples we’re interested in studying and therefore must be removed. The surface sensitive techniques used can generally be divided into spatially-averaged and local probe instruments. Each analytical tool fundamentally relies on Fermi’s golden rule[61]

𝒲 =2𝜋

ℏ |< 𝑓|ℋ

′_{|𝑖 >|}2_{𝜌 } _{2.1}

where ℋ′is the perturbation matrix between final and initial states and ρ is the density of final states. This gives the effectively constant transition rate between eigenstates of a system for a given perturbation. The application of this golden rule for photoemission and scanning tunneling experiments are presented after an introduction to the experimental requirements for these measurements.

29 Surface science experiments are typically performed in high vacuum (HV) systems where

pressure is on the order of 10-6_{ Torr or less and for measurements ultrahigh vacuum systems are used }
where pressure is less than 10-8_{ Torr. This can be directly seen by considering the kinetic theory of gases }
for the adsorption of molecules on a surface. The time constant to form a monolayer on a surface is given
by:

𝜏 =𝑛0√2𝜋𝑚𝑘BT

𝑃 2.2

where n0 is the number of molecules in a monolayer, m is the mass of the molecule, T is the temperature
and P is the pressure. Thus, it takes approximately 1 second for a monolayer to form at room temperature
in a system at 10-6_{ Torr. This time-constant also depends on the sticking coefficient, between 0 and 1, of }
the molecule and surface and is unique to each system.

Another reason for UHV requirements for experimental measurement techniques can be seen by the mean free path of particles described by the kinetic theory of gasses.

𝜆 =𝑘BT

𝑃𝜎2 2.3

30
The analysis systems in this chapter contain two vacuum chambers separated by a valve lock.
One chamber is used to load samples and can reach HV/UHV conditions, then transferred to a chamber
with analysis instruments in requiring ~10-10_{ Torr or better. HV conditions can be reached with simple }
mechanical pumps. The roughing pump can reach pressure in the 10-3_{ Torr range and operates by an }
iterative process of moving gas from the chamber into an expanded piston cavity which is then sealed,
recompressed, and expelled from the pump. A turbomolecular (“turbo”) pump can then reach HV

conditions by evacuating gas particles with a series of turbine blades spinning at frequencies of ~1500 Hz. Lower pressures can then be reached by wrapping the chamber system with heating tape and covered with aluminum foil (“baking out”) evaporating the water, and other molecules, from the chamber walls. This is a mandatory procedure in order to reach UHV conditions and all analysis chambers are baked out after being exposed to air. The introductory sample loading (“intro”) chamber is often exposed to air and is typically not necessary to bake out. Every experiment and sample have different needs so it is important to take care when using these systems.

Pressure in these systems is measured by either a ‘hot’ ion gauge or ‘cold’ cathode gauge both of which operate based on ionizing the gas molecules of a system. The hot-filamant ion gauge uses

thermionic emission of electrons which are accelerated to a grid and collected by a wire whose current is then coverted to a pressure. The cold-cathode gauge utilizes electric and magnetic fields to trap electrons in a plasma which can then ionize gas molecules on impact and collected at the cathode giving an indirect

31 measurement of the pressure. Accurate measurements of the gas density become difficult at pressures below 10-11 Torr which is beyond our experimental capabilities in this lab. The hot ion gauge is sufficient for HV/UHV conditions and the cold gauge is sufficient for HV conditions.

The samples studied in this thesis are vdW layered materials allowing them to be cleaved along a natural crystal plane (perpendicular to the c-axis) ideally creating an atomically flat sample. Visual inspection of the TI sample should indicate the quality of the cleave by the shininess. While this process can produce macroscopic atomically flat regions, there are always unit cell steps which can be verified by scanning probe microscopy.

Partial cleaves of the unit cell can also happen as well and the environment in which a TI is cleaved has been shown to result in coexisting surface terminations. It is therefore best to perform cleaves in vacuum to maximize the probability of a good cleave. In the case of other samples, such as Cr(001), cycles of annealing (Figure 2.1) and ion radiation are used with various recipes in order to produce clean surfaces.

Molecules are thermally sublimed onto a substrate surface through a process called Organic Molecule Beam Deposition (OMBD). Powder of the molecule is placed in a quartz crucible which is wrapped in Tantalum wire and sealed in a vacuum chamber. Current is then passed through the wire with an external power supply connected via feedthroughs heating the wire and crucible. Water and other impurities are expelled from the powder (outgassed) prior to the powder subliming and this process can vary in time length depending on the molecule. A quartz crystal microbalance is often used to establish

32 the molecular flux. It consists of an oscillating (~8 MHz) Au crystal where the change in frequency of oscillation is used to compute the amount of deposited molecules. This generates a nominal value for the thickness of the molecular film which then needs to be verified experimentally.

**2.2 Photoelectron Spectroscopy Theory **

The techniques discussed in this section are X-ray photoelectron spectroscopy, which can

determine near-surface chemical compositions, and angle-resolved photoelectron spectroscopy (ARPES), which maps the emitted photoelectrons as a function of their energy and momentum. Photoelectron spectroscopy (PES) is the general term for the technique that utilizes Einstein’s fundamental photoelectric equation relating a photon of energy, hν, and the maximum kinetic energy of the emitted electrons,

𝐸_{𝑘𝑖𝑛}𝑚𝑎𝑥, to the minimum energy required to remove the electron from a solid (work function) ϕ :

𝐸𝑘𝑖𝑛𝑚𝑎𝑥 = ℎ𝜈 − ϕ 2.4